DOI: 10.17188/1726732
title: Materials Data on Li3Mn4(P2O7)4 by Materials Project

description: Li3Mn4(P2O7)4 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are six inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded to four O2- atoms to form LiO4 tetrahedra that share a cornercorner with one MnO6 octahedra, corners with four PO4 tetrahedra, and an edgeedge with one LiO4 tetrahedra. The corner-sharing octahedral tilt angles are 71°. There are a spread of Li–O bond distances ranging from 1.86–1.98 Å. In the second Li1+ site, Li1+ is bonded to four O2- atoms to form LiO4 tetrahedra that share a cornercorner with one MnO6 octahedra and corners with four PO4 tetrahedra. The corner-sharing octahedral tilt angles are 37°. There are a spread of Li–O bond distances ranging from 1.89–2.02 Å. In the third Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one MnO6 octahedra. There are a spread of Li–O bond distances ranging from 1.85–2.17 Å. In the fourth Li1+ site, Li1+ is bonded to four O2- atoms to form LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of Li–O bond distances ranging from 1.84–1.99 Å. In the fifth Li1+ site, Li1+ is bonded to five O2- atoms to form distorted LiO5 trigonal bipyramids that share corners with five PO4 tetrahedra and an edgeedge with one MnO6 octahedra. There are a spread of Li–O bond distances ranging from 1.81–2.57 Å. In the sixth Li1+ site, Li1+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Li–O bond distances ranging from 1.89–2.54 Å. There are eight inequivalent Mn+3.25+ sites. In the first Mn+3.25+ site, Mn+3.25+ is bonded to six O2- atoms to form distorted MnO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one MnO6 octahedra. There are a spread of Mn–O bond distances ranging from 1.95–2.53 Å. In the second Mn+3.25+ site, Mn+3.25+ is bonded to six O2- atoms to form distorted MnO6 octahedra that share corners with two LiO4 tetrahedra, corners with four PO4 tetrahedra, an edgeedge with one MnO6 octahedra, and an edgeedge with one PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.94–2.48 Å. In the third Mn+3.25+ site, Mn+3.25+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Mn–O bond distances ranging from 1.91–2.35 Å. In the fourth Mn+3.25+ site, Mn+3.25+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.91–2.36 Å. In the fifth Mn+3.25+ site, Mn+3.25+ is bonded to six O2- atoms to form distorted MnO6 octahedra that share corners with six PO4 tetrahedra, an edgeedge with one LiO5 trigonal bipyramid, and an edgeedge with one MnO5 trigonal bipyramid. There are a spread of Mn–O bond distances ranging from 1.90–2.47 Å. In the sixth Mn+3.25+ site, Mn+3.25+ is bonded to five O2- atoms to form distorted MnO5 trigonal bipyramids that share corners with five PO4 tetrahedra and an edgeedge with one MnO6 octahedra. There are a spread of Mn–O bond distances ranging from 1.90–2.20 Å. In the seventh Mn+3.25+ site, Mn+3.25+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Mn–O bond distances ranging from 1.96–2.58 Å. In the eighth Mn+3.25+ site, Mn+3.25+ is bonded to six O2- atoms to form distorted MnO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of Mn–O bond distances ranging from 1.94–2.52 Å. There are sixteen inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two MnO6 octahedra, a cornercorner with one PO4 tetrahedra, a cornercorner with one LiO5 trigonal bipyramid, and a cornercorner with one MnO5 trigonal bipyramid. The corner-sharing octahedra tilt angles range from 48–56°. There are a spread of P–O bond distances ranging from 1.49–1.61 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedral tilt angles are 29°. There are a spread of P–O bond distances ranging from 1.49–1.61 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedral tilt angles are 53°. There are a spread of P–O bond distances ranging from 1.51–1.60 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three MnO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 21–54°. There are a spread of P–O bond distances ranging from 1.53–1.63 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three MnO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 29–46°. There are a spread of P–O bond distances ranging from 1.51–1.62 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, a cornercorner with one PO4 tetrahedra, a cornercorner with one MnO5 trigonal bipyramid, and an edgeedge with one MnO6 octahedra. The corner-sharing octahedral tilt angles are 53°. There are a spread of P–O bond distances ranging from 1.51–1.59 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, a cornercorner with one PO4 tetrahedra, and a cornercorner with one MnO5 trigonal bipyramid. The corner-sharing octahedra tilt angles range from 56–63°. There are a spread of P–O bond distances ranging from 1.48–1.60 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 32–55°. There are a spread of P–O bond distances ranging from 1.52–1.59 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedral tilt angles are 34°. There are a spread of P–O bond distances ranging from 1.50–1.60 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedral tilt angles are 63°. There are a spread of P–O bond distances ranging from 1.48–1.61 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, a cornercorner with one PO4 tetrahedra, and a cornercorner with one LiO5 trigonal bipyramid. The corner-sharing octahedral tilt angles are 49°. There are a spread of P–O bond distances ranging from 1.51–1.60 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, a cornercorner with one PO4 tetrahedra, and a cornercorner with one LiO5 trigonal bipyramid. The corner-sharing octahedra tilt angles range from 31–49°. There are a spread of P–O bond distances ranging from 1.52–1.62 Å. In the thirteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, a cornercorner with one PO4 tetrahedra, and a cornercorner with one LiO5 trigonal bipyramid. The corner-sharing octahedra tilt angles range from 30–51°. There are a spread of P–O bond distances ranging from 1.51–1.62 Å. In the fourteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two MnO6 octahedra, a cornercorner with one PO4 tetrahedra, corners with two LiO4 tetrahedra, and a cornercorner with one MnO5 trigonal bipyramid. The corner-sharing octahedra tilt angles range from 51–57°. There are a spread of P–O bond distances ranging from 1.51–1.60 Å. In the fifteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one LiO4 tetrahedra, a cornercorner with one PO4 tetrahedra, and a cornercorner with one MnO5 trigonal bipyramid. The corner-sharing octahedral tilt angles are 33°. There are a spread of P–O bond distances ranging from 1.50–1.60 Å. In the sixteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share a cornercorner with one MnO6 octahedra, a cornercorner with one PO4 tetrahedra, and a cornercorner with one LiO5 trigonal bipyramid. The corner-sharing octahedral tilt angles are 60°. There are a spread of P–O bond distances ranging from 1.48–1.61 Å. There are fifty-six inequivalent O2- sites. In the first O2- site, O2- is bonded in a distorted bent 120 degrees geometry to two Li1+ and one P5+ atom. In the second O2- site, O2- is bonded in a bent 120 degrees geometry to one Mn+3.25+ and one P5+ atom. In the third O2- site, O2- is bonded in a 3-coordinate geometry to two Mn+3.25+ and one P5+ atom. In the fourth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one Mn+3.25+ and one P5+ atom. In the fifth O2- site, O2- is bonded in a bent 150 degrees geometry to two P5+ atoms. In the sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one Mn+3.25+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a trigonal planar geometry to one Li1+, one Mn+3.25+, and one P5+ atom. In the eighth O2- site, O2- is bonded in a bent 120 degrees geometry to one Li1+ and one P5+ atom. In the ninth O2- site, O2- is bonded in a bent 150 degrees geometry to two P5+ atoms. In the tenth O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+ and one P5+ atom. In the eleventh O2- site, O2- is bonded in a 3-coordinate geometry to two Mn+3.25+ and one P5+ atom. In the twelfth O2- site, O2- is bonded in a bent 150 degrees geometry to one Mn+3.25+ and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a water-like geometry to one Mn+3.25+ and one P5+ atom. In the fourteenth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Mn+3.25+ and one P5+ atom. In the fifteenth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Mn+3.25+ and one P5+ atom. In the sixteenth O2- site, O2- is bonded in a water-like geometry to one Mn+3.25+ and one P5+ atom. In the seventeenth O2- site, O2- is bonded in a bent 150 degrees geometry to one Mn+3.25+ and one P5+ atom. In the eighteenth O2- site, O2- is bonded in a 2-coordinate geometry to two Mn+3.25+ and one P5+ atom. In the nineteenth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to two P5+ atoms. In the twentieth O2- site, O2- is bonded in a 2-coordinate geometry to one Li1+, one Mn+3.25+, and one P5+ atom. In the twenty-first O2- site, O2- is bonded in a bent 120 degrees geometry to one Li1+ and one P5+ atom. In the twenty-second O2- site, O2- is bonded in a trigonal planar geometry to one Li1+, one Mn+3.25+, and one P5+ atom. In the twenty-third O2- site, O2- is bonded in a bent 150 degrees geometry to one Mn+3.25+ and one P5+ atom. In the twenty-fourth O2- site, O2- is bonded in a bent 150 degrees geometry to two P5+ atoms. In the twenty-fifth O2- site, O2- is bonded in a 3-coordinate geometry t